Materials Letters 102–103 (2013) 62–64
Contents lists available at SciVerse ScienceDirect
Materials Letters journal homepage: www.elsevier.com/locate/matlet
In situ synchrotron diffraction of the solidiﬁcation of Mg4Y3Nd D. Tolnai n, C.L. Mendis, A. Stark, G. Szakács, B. Wiese, K.U. Kainer, N. Hort Institute of Materials Research, Helmholtz-Zentrum Geesthacht, Max-Planck Str. 1, D-21502 Geesthacht, Germany
art ic l e i nf o
a b s t r a c t
Article history: Received 28 February 2013 Accepted 22 March 2013 Available online 30 March 2013
In situ synchrotron diffraction experiments were performed during the solidiﬁcation of a Mg4Y3Nd alloy. The material was melted and solidiﬁed inside a sealed stainless steel crucible in the chamber of a Bähr 805 A/D dilatometer. The sample was heated up to 680 1C and kept at this temperature for 5 min to ensure it is molten. Afterwards it was cooled down to the fully solidiﬁed state with a cooling rate of 10 K/ min. During the T(t) program diffraction patterns were acquired continuously in every 25 s (∼5 K). The forming phases were identiﬁed as α-Mg at 625 1C, Mg12Nd and Mg14Y4Nd at 545 1C, and Mg24Y5 at 320 1C. The experimental results were correlated with simulations based on thermodynamic databases. & 2013 Elsevier B.V. All rights reserved.
Keywords: Mg alloys Solidiﬁcation In situ Synchrotron diffraction
1. Introduction Mg–RE based alloys are attractive for structural  as well as for biomaterial applications  due to the good combination of mechanical and corrosion properties. Commercial Mg–Y–Nd based alloys, such as WE43 and WE54 form an important class of alloys used in elevated temperature applications with superior mechanical properties at both room and elevated temperatures . The WE54 and WE43 alloys are conventionally used in the T6 condition. The age hardening response as well as the precipitation sequence and crystal structures of the resultant phases investigated previously [4–7]. The intermetallic particles found in the as-cast Mg5Y2Nd (wt%) and Mg4Y2Nd (wt%) alloys have been characterized, with transmission electron microcopy to be a ternary phase with a face centered cubic crystal structure with a¼ 2.223 nm and a composition of Mg14Nd2Y  or Mg15Nd2Y . The macroscopic mechanical properties of multiphase materials depend strongly on the chemical composition, volume fraction and spatial distribution of the intermetallic phases . The thermodynamic databases and binary phase diagrams  provide information on the presumed solidiﬁcation paths of the simple alloy systems. Based on these databases, the resultant microstructure can be modeled . The majority of the commercial Mg alloys are not binary, but containing more than one alloying addition resulting in complex inter metallics. For these complex phases the information in the simulation databases is limited. Thus the simulation of the experimentally observed microstructure and modeling of the solidiﬁcation sequence is not feasible in every case due to the lack of available data. The continuous development of the X-ray acquisition systems at synchrotron sources provides a unique tool to characterize the
Corresponding author. Tel.: +49 4152 871974; fax: +49 4152 871909. E-mail address: [email protected]
0167-577X/$ - see front matter & 2013 Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.matlet.2013.03.110
phase formation and evolution during the solidiﬁcation in situ. Recording the diffraction patterns while cooling the alloy system down, allows identifying the internal phases, to determine their solidiﬁcation sequence [12,13] and to use these results as experimental validation of the existing thermodynamic databases and in certain cases contribute to their further development. The present study reports results on the in situ synchrotron diffraction during solidiﬁcation of a Mg4Y3Nd alloy, and their comparison with the existing thermodynamic data on this system. 2. Materials and methods The alloy Mg4Y3Nd (wt%) was chosen for the experiments, as it is of particular interest in structural and in biomaterial applications. The microstructure of the direct chill cast alloy was examined with a Carl Zeiss Gemini Ultra 55 scanning electron microscope (SEM) operating at 15 kV. The samples for the synchrotron diffraction measurements were cut into small cubes and encapsulated in steel crucibles. The experiments were carried out at the HARWI II beamline of the Hamburger Synchrotronstrahlungslabor (HASYLAB) at the Deutsches Elektronen-Synchrotron (DESY). The measurements were performed in the chamber of a DIL 805 A/D (Bähr-Thermoanalyse GmbH, Hüllhorst, Germany) dilatometer the experimental setup is shown in Fig. 1. During the tests the samples were held in a sealed stainless steel crucible in order to hold the molten metal and to isolate it from the surrounding atmosphere. The dilatometer has been modiﬁed to meet the requirements of in situ synchrotron measurements. The two windows on the sides are covered by Kapton foils, to prevent interference with the X-ray beam. The induction coil is modiﬁed so the beam to only passes through the sample . The temperature was regulated by a type S thermocouple welded on the steel crucible
D. Tolnai et al. / Materials Letters 102–103 (2013) 62–64
Fig. 1. Experimental setup of the in situ solidiﬁcation experiment inside the chamber of a Bähr 805 A/D dilatometer modiﬁed for in situ synchrotron measurements. The windows on the sides are covered by Kapton foil, while the coil is opened, for the beam to pass through the sample.
containing the sample. The heating and cooling was performed in Ar ﬂow. To melt the samples the system was heated up to 680 1C, held for 5 min and then cooled to 180 1C at a cooling rate of 10 K/ min. The in situ diffraction experiment was done in transmission geometry using a beam cross section of 1 1 mm2. In order to penetrate the sample, high-energy X-rays were used with a photon energy of 100 keV, corresponding to a wavelength of λ¼0.0124 nm. During the experiment the Debye–Scherrer diffraction rings were recorded in every 25 s (∼5 K) with an acquisition time of 2 s by a mar555 ﬂatpanel detector (Marresearch GmbH, Norderstedt, Germany) with an area of 3070 2560 pixels with a pixel size of 140 mm². Conventional diffraction patterns (line proﬁles) were achieved by an azimuthal integration of the Debye–Scherrer rings. The line proﬁles were indexed based on the peak positions obtained by CaRIne Crystallography 3.1. The thermodynamic simulation of the solidiﬁcation was carried out with the software Pandat 8.1.
Fig. 2. Secondary electron micrograph of the investigated Mg4Y3Nd alloy in as-cast condition.
Fig. 3. Sequence of XRD line diagrams at different temperatures obtained by the integration of the diffraction patterns recorded during solidiﬁcation. (Wavelength λ¼ 0.0124 nm).
3. Results and discussion The secondary electron micrograph is shown in Fig. 2. The microstructure consists of α-Mg dendrites and intermetallic particles with Y and Nd. The XRD line diagrams resulting from the azimuthal integration of the 2D diffraction patterns are shown in Fig. 3. Based on the peak positions the solidiﬁcation sequence of the phases can be determined with a temperature resolution of ∼5 1C. The solidiﬁcation starts with the nucleation and growth of the α-Mg dendrites at a measured temperature of 625 1C. As the cooling advances the dendrites are followed by the Nd containing intermetallic phases. The binary Mg12Nd and the ternary Mg14Y4Nd phases are ﬁrst observed at 545 1C. Finally, solidiﬁcation of Mg24Y5 can be observed at 320 1C. The resulting section of the ternary phase diagram obtained by Pandat at an Nd content of 3 wt% is shown in Fig. 4. The vertical line corresponds to a Y content of 4 wt%. According to the thermodynamic database the α-Mg dendrites initiate at 639 1C. They are followed by the Mg41Nd5 phase at 538 1C, while the solidiﬁcation ends with the Mg24Y5 phase at 316 1C. The solidiﬁcation of any ternary phase is not predicted to be an expected phase by the thermodynamic database. The determination of the solidiﬁcation sequence by in situ synchrotron diffraction has some limitations. A compromise must be made between the cooling rate and the acquisition time. The crystallographic orientation of the solidifying grains plays a vital role. As these grains ﬂoat in the melt without ﬁxed orientation their detection is difﬁcult. It is likely that the α-Mg grains can be detected for the ﬁrst time as the system reaches the dendrites
Fig. 4. Section of the ternary Mg–Y–Nd phase diagram at a Nd content of 3 wt%, calculated by Pandat 8.1.
coherency point, the temperature where a continuous dendrite skeleton is built up. Despite these limitations, the onset temperatures, obtained experimentally by in situ diffraction and that predicted theoretically from the thermodynamic calculations,
D. Tolnai et al. / Materials Letters 102–103 (2013) 62–64
for the solidiﬁcation of different phases correlate reasonably well. Instead of Mg41Nd5, Mg12Nd was found, while the ternary intermetallic phase Mg14Y4Nd was only shown experimentally and not predicted by the thermodynamic simulations performed with Pandat software. This can be attributed to either the limited information available in the database, or the Mg14Y4Nd phase is thermodynamically meta-stable.
4. Conclusions In conclusion, in situ solidiﬁcation experiments were performed with a Bähr 805 A/D dilatometer, on a Mg4Y3Nd alloy by synchrotron diffraction, for the ﬁrst time. During cooling with 10 K/min from 680 1C to 180 1C, the solidiﬁcation sequence could be determined experimentally. First α-Mg solidiﬁes at a temperature of 625 1C followed by the solidiﬁcation of the intermetallic particles; Mg12Nd and Mg14Y4Nd at 545 1C and ﬁnally the Mg24Y5 phase at a temperature of 320 1C. The results are in correlation with the results obtained by the thermodynamic calculations performed with Pandat 8.1. In situ synchrotron diffraction reveals the presence of the ternary Mg14Y4Nd phase and the onset of its solidiﬁcation at 545 1C which could not be predicted by the simulations.
Acknowledgments The authors acknowledge the Deutsches Elektronen-Synchrotron for the provision of synchrotron radiation facilities in the framework of the proposal II-20100225. References  Rokhlin LL. Magnesium alloys containing rare earth metals, structure and properties. Taylor & Francis; 2003.  Hort N, Huang Y, Fechner D, Störmer M, Blawert C, Witte F, et al. Acta Biomat 2010;6:1714.  Barucca G, Ferragut R, Fiori F, Lussana D, Mengucci P, Moria F, et al. Acta Mat 2011;59:4151.  Antion C, Donnadieu P, Perrad F, Deschamps A, Tassin C, Pisch A. Acta Mat 2003;51:5335.  Nie JF, Muddle BC. Acta Mat 2000;48:1691.  Apps PJ, Karimzadeh H, King JF, Lorimer GW. Scripta Mat 2003;48:1023.  Apps PJ, Karimzadeh H, King JF, Lorimer GW. Scripta Mat 2003;48:475.  H Karimzadeh PhD thesis. Manchester University. United Kingdom; 1985.  Requena G, Garcés G, Asghar Z, Marks E, Staron P, Cloetens P. Adv Eng Mat 2011;13:674.  Massalski TB. Binary alloy phase diagrams. ASM International Materials Park; 1990.  Boettinger WJ, Warren JA, Beckermann C, Karma A. An Rev Mat Res 2002;32:164.  Babu SS, Elmer JW, Vitek JM, David SA. Acta Mat 2002;50:4763.  Shuleshova O, Moritz DH, Voss A, Löser W. Intermetallics 2011;19:688.  Staron P, Fischer T, Lippmann T, Stark A, Daneshpour S, Schnubel D, et al. Adv Eng Mat 2011;13:658.